DNA-templated synthesis of PtAu bimetallic nanoparticle/graphene nanocomposites and their application in glucose biosensor
© Leng et al.; licensee Springer. 2014
Received: 26 November 2013
Accepted: 19 January 2014
Published: 27 February 2014
In this paper, single-stranded DNA (ss-DNA) is demonstrated to functionalize graphene (GR) and to further guide the growth of PtAu bimetallic nanoparticles (PtAuNPs) on GR with high densities and dispersion. The obtained nanocomposites (PtAuNPs/ss-DNA/GR) were characterized by transmission electron microscopy (TEM), energy-dispersive X-ray spectrometer (EDS), and electrochemical techniques. Then, an enzyme nanoassembly was prepared by self-assembling glucose oxidase (GOD) on PtAuNP/ss-DNA/GR nanocomposites (GOD/PtAuNPs/ss-DNA/GR). The nanocomposites provided a suitable microenvironment for GOD to retain its biological activity. The direct and reversible electron transfer process between the active site of GOD and the modified electrode was realized without any extra electron mediator. Thus, the prepared GOD/PtAuNP/ss-DNA/GR electrode was proposed as a biosensor for the quantification of glucose. The effects of pH, applied potential, and temperature on the performance of the biosensor were discussed in detail and were optimized. Under optimal conditions, the biosensor showed a linearity with glucose concentration in the range of 1.0 to 1,800 μM with a detection limit of 0.3 μM (S/N = 3). The results demonstrate that the developed approach provides a promising strategy to improve the sensitivity and enzyme activity of electrochemical biosensors.
KeywordsGraphene PtAu bimetallic nanoparticles Glucose oxidase Biosensor Glucose
It is well known that the diabetes mellitus is one of the leading causes of death and disability in the world which can be easily diagnosed and managed by the determination of blood glucose . The great importance of glucose monitoring leads to a considerable amount of fascinating research and innovative detection strategies. Among various glucose detection methods, such as spectrophotometric , chemiluminescence , and electrochemical methods [4–6], the amperometric electrochemical biosensor based on glucose oxidase (GOD) has played a leading role in the move of simple one-step blood sugar testing. Since the development of the first glucose biosensor, improvement of the response performances of enzyme electrodes has continued to be the main focus of biosensor research . In particular, research for new materials and methods for immobilizing enzyme is still a very important subject to get more active and stable biosensors.
GR, with a two-dimensional (2D) sp2-hybridized carbon structure in a single-atom-thick sheet, has rapidly emerged as one of the most attractive materials [8, 9]. Due to its unique physical and chemical properties, such as high surface area, excellent conductivity, good chemical stability, and strong mechanical strength, GR provides an ideal base for electronics, electric devices, and biosensors [10–17]. Recently, GR-based hybrids are of scientific and industrial interest due to the synergistic contribution of two or more functional components. With appropriate designs, nanocomposites can exhibit the beneficial properties of each parent constituent, producing a material with improved performance. Up to now, various materials have been incorporated with GR layers, including conducting polymers , carbon nanospheres , metal nanoparticles (NPs) , and ionic liquid , to construct electrochemical sensors. Among them, metal NPs have received a great deal of interest on account of their unique electronic, chemical, and optical properties. Because PtNPs and AuNPs could provide a suitable microenvironment for biomolecule immobilization and facilitate electron transfer between the immobilized protein and PtNPs and AuNPs, they have been widely applied in immunosensors and biosensors [22–24]. On the basis of the outstanding physical and chemical properties of PtNPs, AuNPs, and GR composites, it is highly desirable that a hybrid composed of PtAu bimetallic nanoparticles (PtAuNPs) and GR could be used as the sensing platform in electrochemical biosensors.
To date, GR-metal hybrids are primarily prepared by in situ growth method. However, it is difficult to grow small and uniformly distributed metal NPs on GR surface. In addition, the resulting GR-metal hybrids are mostly in the form of precipitate and not suitable for applications requiring well-dispersed materials. In order to obtain water-soluble GR-based hybrids, various molecules including polymers and surfactants have been recently utilized to functionalize GR [25, 26] as supports for metal NPs, but great challenges still remain in rationally functionalizing GR as a superior support for significantly improved electrochemical performance. Deoxyribonucleic acid (DNA) is a well-known natural biological macromolecule, which has regularly arranged functional groups and well-developed chemistries for different specific modifications . Recently, the combination of DNA with carbon-based nanomaterials such as carbon nanotubes (CNTs) through π-stacking for the development of novel biomaterials and devices has attracted great attention in the field of DNA transporters  and field-effect transistors . Also, DNA can be used as an inexpensive, well-characterized, controllable, and easily adaptable material to construct defined hybrid nanostructures [30, 31]. Therefore, DNA modification is expected to eliminate the aggregation of GR for high dispersion efficiency, and its well-developed chemistries may direct the growth of metal NPs with uniform distribution on GR.
Experimental device and reagent
A transmission electron microscopy (TEM) image was taken with a JEM-3010 transmission electron microscope (JEOL Co., Ltd., Tokyo, Japan). The cyclic voltammetric, amperometric, and electrochemical impedance spectroscopy measurements were carried out on a CHI 760B electrochemical workstation (CH Instruments, Inc., Shanghai, China). Electrochemical impedance spectroscopy was performed in a 5 mM K3Fe(CN)6/K4Fe(CN)6 (1:1) mixture with 0.1 M KCl at a formal potential of 240 mV using an alternating voltage of 5 mV. The frequency range was from 1 Hz to 100 kHz. A three-electrode cell (10 mL) was used with the modified glassy carbon (GC) electrode as the working electrode, a saturated calomel electrode (SCE) as the reference electrode, and platinum foil electrode as the counter electrode. All potentials were measured versus the SCE, and all experiments were carried out at room temperature.
Native double-stranded DNA (ds-DNA) from calf thymus and GOD were purchased from Sigma Chemical (St. Louis, MO, USA). Graphite powder (99.95%, 325 mesh), hydrogen peroxide solution (30 wt.% aqueous), and hydrazine solution (50 wt.%) were purchased from the Beijing Chemical Reagent factory (Beijing, China) and used as received. All other reagents were of analytical grade, and double-distilled water was used throughout the experiments.
Preparation of graphite oxide, ss-DNA/GR, and PtAuNP/ss-DNA/GR nanocomposite
Graphite oxide (GO) was prepared from graphite powder according to the method of Hummers , and the PtAuNP/ss-DNA/GR nanocomposites were synthesized according to the reported method with a slight modification . Briefly, an aqueous solution of ds-DNA was first heated at 95°C for 2 h to obtain an aqueous solution of ss-DNA. GO (60 mg) was dispersed in water (60 mL) containing 6 mg mL-1 ss-DNA by ultrasonic treatment for 30 min. Then, a 0.02 M H2PtCl6 and 0.02 M HAuCl4 solution was added and stirred for 30 min. The mixture was then heated to reflux at 100°C for 4 h to prepare the PtAuNP/ss-DNA/GR nanocomposite. After cooling to room temperature, the resulting materials were then centrifuged and washed three times with distilled water. The as-prepared PtAuNP/ss-DNA/GR nanocomposite was water soluble and could be stored as an aqueous solution at a concentration of 2 mg mL-1. Additionally, the preparation of ss-DNA/GR, PtNP/ss-DNA/GR, and AuNP/ss-DNA/GR composites was done in a similar procedure except that there was no addition of H2PtCl6 or HAuCl4.
Fabrication of GOD/PtAuNP/ss-DNA/GR modified electrode
To prepare the enzyme-modified electrode, a bare GC electrode was polished to be mirror-like with alumina powder (0.05 μm), then washed successively with double-distilled water, anhydrous ethanol, and double-distilled water in an ultrasonic bath, and was dried under N2 before use. In order to accomplish electrode coating, 5- μL aliquots of the PtAuNP/ss-DNA/GR solution were dropped and dried on the surface of a GC electrode. The PtAuNP/ss-DNA/GR-modified electrode was then immersed in a GOD working solution (10 mg mL-1, 0.1 M PBS) for about 8 h at 4°C to immobilize GOD on the surface of the electrode (Figure 1). Finally, the fabricated glucose biosensor (GOD/PtAuNPs/ss-DNA/GR) was rinsed thoroughly with water to wash away the loosely adsorbed enzyme molecules. The fabricated glucose biosensor was stored at 4°C in a refrigerator when not in use. For comparison, GOD/PtNPs/ss-DNA/GR, GOD/AuNPs/ss-DNA/GR, and GOD/ss-DNA/GR were prepared through similar procedures.
Results and discussion
Characterization of ss-DNA/GR and PtAuNP/ss-DNA/GR nanocomposites
Electrochemical impedance spectroscopy characterization of self-assembly process
Electrochemical properties of GOD/PtAuNP/ss-DNA/GR modified electrode
According to the reaction above, there is a linear relationship between the amount of glucose increase and the dissolved O2 decrease, that is, a model of the glucose amperometric biosensor could be constructed by detecting the decrease of the reduction peak current of dissolved O2 to indicate the concentration of glucose.
Optimization of experimental conditions
The applied potential is an important parameter that affects the sensitivity of the biosensor. Figure 5B displays the dependence of applied potential on the amperometric response of the biosensor to 0.1 mM glucose in PBS (pH 7.0). When the applied potential was changed from 0 to -0.35 V, the maximum response current was observed at -0.2 V. To obtain high sensitivity and to minimize possible interferences, -0.2 V was chosen as the optimum applied potential for further investigations.
The effect of temperature on the amperometric response of glucose was also studied. The biosensor was immersed into the buffer solution at a given temperature for 10 min before amperometric detection, and then the response of the electrode was measured at this temperature. As shown in Figure 5C, the electrochemical response increases with increasing temperature from 25°C to 35°C and then decreases as the temperature further increased. The sharp decrease of the response was due to the denaturation of GOD at high temperatures. Although the response of the biosensor was greatest at 35°C, for practical reasons, it was suggested that room temperature be used to simplify the experimental procedure and prolong the useful lifetime of the biosensor given that most enzymes can be easily denatured at high temperature.
Amperometric sensing of glucose
Selectivity, reproducibility, and stability of the biosensor
Interference studies at the GOD/PtAuNP/ss-DNA/GR modified electrode
Response current (μA)
Glucose (1 mM)
Ascorbic acid (1 mM)
Dopamine (1 mM)
Uric acid (1 mM)
The reproducibility and repeatability of the developed biosensor were determined. In a series of 10 biosensors prepared in the same way, a relative standard deviation (RSD) of 5.1% was obtained toward 0.1 mM glucose, indicating the reliability of the method. A set of 10 different amperometric measurements for 0.1 mM glucose with a single sensor yielded an RSD of 4.6%.
The stability of the glucose biosensor was explored. The proposed biosensor was stored at 4°C in the refrigerator. The response to 0.1 mM glucose was tested each week; after 21 days of storage, the response of the biosensor only had a decrease of 5.5% compared to the initial response, which shows long-term stability. Such a high stability could be attributed to the favorable microenvironment that maintains the GOD activity and prevents the leakage of enzyme.
Real sample analysis
Amperometric determination of glucose in human blood serum samples
In this work, a novel electrochemical GOD biosensor based on PtAuNP/ss-DNA/GR nanocomposites was developed for the determination of glucose. The bionanocomposite film provided a suitable microenvironment, which could effectively present a large loading amount of enzyme and enhanced the direct electron transfer between the enzyme's active sites and the electrode. The modified electrode exhibited excellent analytical performance with wide linear range, low detection limit, and good selectivity for measuring glucose. Therefore, the composite of PtAuNPs/ss-DNA/GR is a good material platform, promising for construction of the third-generation enzyme biosensor, biofuel cells, and bioelectrochemical devices.
JL is an undergraduate student at Jiangxi Agricultural University. W-MW, L-ML, LB, and X-LQ are teachers at Jiangxi Agricultural University.
energy-dispersive X-ray spectrometer
PtAu bimetallic nanoparticles
transmission electron microscopy.
This work was supported by the National Natural Science Foundation of China (51302117), the Natural Science Foundation of Jiangxi Province (20122BAB213007), State Key Laboratory of Chemical Biosensing & Chemometrics (201108), and Jiangxi Provincial Department of Education (GJJ13258).
- Zheng BZ, Xie S, Qian L, Yuan HY, Xiao D, Choi M: Gold nanoparticles-coated eggshell membrane with immobilized glucose oxidase for fabrication of glucose biosensor. Sens Actuators B 2011, 152: 49–55. 10.1016/j.snb.2010.09.051View ArticleGoogle Scholar
- Han AX, Wu GS, Liang Q, Zhang FS: Direct spectrophotometric determination of the blood glucose by the method of conjugation enzyme. Chin J Anal Chem 2003, 31: 1417–1420.Google Scholar
- Liu XQ, Niu W, Li HJ, Han S, Hu LZ, Xu GB: Glucose biosensor based on gold nanoparticle-catalyzed luminol electrochemiluminescence on a three-dimensional sol–gel network. Electrochem Commun 2008, 10: 1250–1253. 10.1016/j.elecom.2008.06.009View ArticleGoogle Scholar
- Xu CX, Huang KJ, Chen XM, Xiong XQ: Direct electrochemistry of glucose oxidase immobilized on TiO2-graphene/nickel oxide nanocomposite film and its application. J Solid State Electrochem 2012, 16: 3747–3752. 10.1007/s10008-012-1813-5View ArticleGoogle Scholar
- Li J, Yang ZJ, Xu Q, Qu QS, Hu XY: Tin disulfide nanoflakes decorated with gold nanoparticles for direct electrochemistry of glucose oxidase and glucose biosensing. Microchim Acta 2012, 179: 265–272. 10.1007/s00604-012-0889-zView ArticleGoogle Scholar
- Liu S, Tian JQ, Luo YL, Lu W, Sun XP: Self-assembled graphene platelet-glucose oxidase nanostructures for glucose biosensing. Biosens Bioelectron 2011, 26: 4491–4496. 10.1016/j.bios.2011.05.008View ArticleGoogle Scholar
- Raitman OA, Katz E, Buckmann AF, Willner I: Integration of polyaniline/poly(acrylic acid) films and redox enzymes on electrode supports: an in situ electrochemical/surface plasmon resonance study of the bioelectrocatalyzed oxidation of glucose or lactate in the integrated bioelectrocatalytic systems. J Am Chem Soc 2002, 124: 6487–6496. 10.1021/ja012680rView ArticleGoogle Scholar
- Huang X, Qi XY, Boey F, Zhang H: Graphene-based composites. Chem Soc Rev 2012, 41: 666–686. 10.1039/c1cs15078bView ArticleGoogle Scholar
- Huang X, Yin ZY, Wu SX, Qi XY, He QY, Zhang QC, Yan QY, Boey F, Zhang H: Graphene-based materials: synthesis, characterization, properties, and applications. Small 2011, 7: 1876–1902. 10.1002/smll.201002009View ArticleGoogle Scholar
- Si Y, Samulski ET: Exfoliated graphene separated by platinum nanoparticles. Chem Mater 2008, 20: 6792–6797. 10.1021/cm801356aView ArticleGoogle Scholar
- Yoo EJ, Kim J, Hosono E, Zhou HS, Kudo T, Honma I: Large reversible Li storage of graphene nanosheet families for use in rechargeable lithium ion batteries. Nano Lett 2008, 8: 2277–2282. 10.1021/nl800957bView ArticleGoogle Scholar
- Unnikrishnan B, Palanisamy S, Chen SM: A simple electrochemical approach to fabricate a glucose biosensor based on graphene-glucose oxidase biocomposite. Biosens Bioelectron 2013, 39: 70–75. 10.1016/j.bios.2012.06.045View ArticleGoogle Scholar
- Chen D, Feng H, Li J: Graphene oxide: preparation, functionalization, and electrochemical applications. Chem Rev 2012, 112: 6027–6053. 10.1021/cr300115gView ArticleGoogle Scholar
- Chen D, Tang L, Li J: Graphene-based materials in electrochemistry. Chem Soc Rev 2010, 39: 3157–3180. 10.1039/b923596eView ArticleGoogle Scholar
- Zhang PP, Zhang XY, Zhang SY, Lu X, Li Q, Su ZQ, Wei G: One-pot green synthesis, characterizations, and biosensor application of self-assembled reduced graphene oxide-gold nanoparticle hybrid membranes. J Mater Chem B 2013, 1: 6525–6531. 10.1039/c3tb21270jView ArticleGoogle Scholar
- Qu FL, Lu HM, Yang MH, Deng CY: Electrochemical immunosensor based on electron transfer mediated by graphene oxide initiated silver enhancement. Biosens Bioelectron 2011, 26: 4810–4814. 10.1016/j.bios.2011.06.018View ArticleGoogle Scholar
- Li T, Shu B, Jiang B, Ding L, Qi HZ, Yang MH, Qu FL: Ultrasensitive multiplexed protein biomarker detection based on electrochemical tag incorporated polystyrene spheres as label. Sens Actuators B 2013, 186: 768–773.View ArticleGoogle Scholar
- Ameen S, Akhtar MS, Shin HS: Hydrazine chemical sensing by modified electrode based on in situ electrochemically synthesized polyaniline/graphene composite thin film. Sens Actuators B 2012, 173: 177–183.View ArticleGoogle Scholar
- Wang J, Yin HS, Meng XM, Zhu JY, Ai SY: Preparation of the mixture of graphene nanosheets and carbon nanospheres with high adsorptivity by electrolyzing graphite rod and its application in hydroquinone detection. J Electroanal Chem 2011, 662: 317–321. 10.1016/j.jelechem.2011.08.019View ArticleGoogle Scholar
- Zhou L, Gu H, Wang C, Zhang JL, Lv M, He RY: Study on the synthesis and surface enhanced Raman spectroscopy of graphene-based nanocomposites decorated with noble metal nanoparticles. Colloids Surf A 2013, 430: 103–109.View ArticleGoogle Scholar
- Zhao LJ, Zhao FQ, Zeng BZ: Electrochemical determination of methyl parathion using a molecularly imprinted polymer-ionic liquid-graphene composite film coated electrode. Sens Actuators B 2013, 176: 818–824.View ArticleGoogle Scholar
- Wu H, Wang J, Kang XH, Wang CM, Wang DH, Liu J, Aksay IA, Lin YH: Glucose biosensor based on immobilization of glucose oxidase in platinum nanoparticles/graphene/chitosan nanocomposite film. Talanta 2009, 80: 403–406. 10.1016/j.talanta.2009.06.054View ArticleGoogle Scholar
- Han J, Zhuo Y, Chai YQ, Mao L, Yuan YL, Yuan R: Highly conducting gold nanoparticles-graphene nanohybrid films for ultrasensitive detection of carcinoembryonic antigen. Talanta 2011, 85: 130–135. 10.1016/j.talanta.2011.03.036View ArticleGoogle Scholar
- Zan XL, Fang Z, Wu J, Xiao F, Huo FW, Duan HW: Freestanding graphene paper decorated with 2D-assembly of Au@Pt nanoparticles as flexible biosensors to monitor live cell secretion of nitric oxide. Biosens Bioelectron 2013, 49: 71–78.View ArticleGoogle Scholar
- Lotya M, King PJ, Khan U, De S, Coleman JN: High-concentration, surfactant-stabilized graphene dispersions. ACS Nano 2010, 4: 3155–3162. 10.1021/nn1005304View ArticleGoogle Scholar
- Cai DY, Song M: Recent advance in functionalized graphene/polymer nanocomposites. J Mater Chem 2010, 20: 7906–7915. 10.1039/c0jm00530dView ArticleGoogle Scholar
- Chen SM, Chen SV: The bioelectrocatalytic properties of cytochrome C by direct electrochemistry on DNA film modified electrode. Electrochim Acta 2003, 48: 513–529. 10.1016/S0013-4686(02)00719-3View ArticleGoogle Scholar
- Kam NW, Liu Z, Dai HJ: Functionalization of carbon nanotubes via cleavable disulfide bonds for efficient intracellular delivery of siRNA and potent gene silencing. J Am Chem Soc 2005, 127: 12492–12493. 10.1021/ja053962kView ArticleGoogle Scholar
- Gui EL, Li LJ, Zhang K, Xu YP, Dong XC, Ho XN, Lee PS, Kasim J, Shen ZX, Rogers JA, Mhaisalkar SG: DNA sensing by field-effect transistors based on networks of carbon nanotubes. J Am Chem Soc 2007, 129: 14427–14432. 10.1021/ja075176gView ArticleGoogle Scholar
- Xu SJ, Li LM, Du ZF, Tang LH, Wang Y, Wang TH, Li JH: A netlike DNA-templated Au nanoconjugate as the matrix of the direct electrochemistry of horseradish peroxidase. Electrochem Commun 2009, 11: 327–330. 10.1016/j.elecom.2008.12.002View ArticleGoogle Scholar
- Fang C, Fan Y, Kong JM, Zhang GJ, Linn L, Rafeah S: DNA-templated preparation of palladium nanoparticles and their application. Sens Actuators B 2007, 126: 684–690. 10.1016/j.snb.2007.04.031View ArticleGoogle Scholar
- Hummers WS, Offeman RE: Preparation of graphitic oxide. J Am Chem Soc 1958, 80: 1339–1339. 10.1021/ja01539a017View ArticleGoogle Scholar
- Zhang Q, Qiao Y, Hao F, Zhang L, Wu SY, Li Y, Li JH, Song X: Fabrication of a biocompatible and conductive platform based on a single-stranded DNA/graphene nanocomposite for direct electrochemistry and electrocatalysis. Chem Eur J 2010, 16: 8133–8139. 10.1002/chem.201000684View ArticleGoogle Scholar
- Benedetto A, Au C, Aschner M: Manganese-induced dopaminergic neurodegeneration: insights into mechanisms and genetics shared with Parkinson’s disease. Chem Rev 2009, 109: 4862–4884. 10.1021/cr800536yView ArticleGoogle Scholar
- Razmi H, Mohammad-Rezaei R: Graphene quantum dots as a new substrate for immobilization and direct electrochemistry of glucose. Biosens Bioelectron 2013, 41: 498–504.View ArticleGoogle Scholar
- Liu S, Ju H: Reagentless glucose biosensor based on direct electron transfer of glucose oxidase immobilized on colloidal gold modified carbon paste electrode. Biosens Bioelectron 2003, 19: 177–183. 10.1016/S0956-5663(03)00172-6View ArticleGoogle Scholar
- Yang H, Zhu Y: Size dependence of SiO2particles enhanced glucose biosensor. Talanta 2006, 68: 569–574. 10.1016/j.talanta.2005.04.057View ArticleGoogle Scholar
- Tsai MC, Tsai YC: Adsorption of glucose oxidase at platinum-multiwalled carbon nanotube-alumina-coated silica nanocomposite for amperometric glucose biosensor. Sens Actuators B 2009, 141: 592–598. 10.1016/j.snb.2009.06.016View ArticleGoogle Scholar
- Hu F, Chen S, Wang C, Yuan R, Chai Y, Xiang Y, Wang C: ZnO nanoparticle and multiwalled carbon nanotubes for glucose oxidase direct electron transfer and electrocatalytic activity investigation. J Mol Catal B Enzym 2011, 72: 298–304. 10.1016/j.molcatb.2011.07.005View ArticleGoogle Scholar
- Wang Y, Liu L, Li M, Xu S, Gao F: Multifunctional carbon nanotubes for direct electrochemistry of glucose oxidase and glucose bioassay. Biosens Bioelectron 2011, 30: 107–111. 10.1016/j.bios.2011.08.038View ArticleGoogle Scholar
- Gutierrez F, Rubianes MD, Rivas GA: Dispersion of multi-wall carbon nanotubes in glucose oxidase: characterization and analytical applications for glucose biosensing. Sens Actuators B 2012, 161: 191–197. 10.1016/j.snb.2011.10.010View ArticleGoogle Scholar
- Kang X, Wang J, Aksay IA, Lin Y: Glucose oxidase-graphene-chitosan modified electrode for direct electrochemistry and glucose sensing. Biosens Bioelectron 2009, 25: 901–905. 10.1016/j.bios.2009.09.004View ArticleGoogle Scholar
- Xu L, Zhu Y, Yang XL, Li CZ: Amperometric biosensor based on carbon nanotubes coated with polyaniline/dendrimer-encapsulated Pt nanoparticles for glucose detection. Mater Sci Eng C 2009, 29: 1306–1310. 10.1016/j.msec.2008.10.031View ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly credited.